Deviation Between the Chemistry of Ce(IV) and Pu(IV) and Routes to Ordered and Disordered Heterobimetallic 4f/5f and 5f/5f Phosphonates
Juan Diwu; Shuao Wang; Justin J. Good; Victoria H. DiStefano; Thomas E. Albrecht-Schmitt; Inorganic Chemistry 50 (2011) 4842–4850; doi:10.1021/ic200006m

data_4325180
_publ_section_title
;
 Deviation Between the Chemistry of Ce(IV) and Pu(IV) and Routes to
 Ordered and Disordered Heterobimetallic 4f/5f and 5f/5f Phosphonates
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              4842
_journal_page_last               4850
_journal_paper_doi               10.1021/ic200006m
_journal_volume                  50
_journal_year                    2011
_chemical_formula_moiety         (UO2)Ce(H2O)[C6H4(PO3H)2]2.H2O
_chemical_formula_sum            'C12 H10 Ce O16 P4 U'
_chemical_formula_weight         912.23
_chemical_name_common
'Uranyl Cerium bimetallic 1,2-Phenyldiphosphonate'
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           61
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2ab'
_symmetry_space_group_name_H-M   'P b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   15.028(4)
_cell_length_b                   14.959(4)
_cell_length_c                   20.254(6)
_cell_measurement_reflns_used    3785
_cell_measurement_temperature    100(2)
_cell_measurement_theta_max      27.53
_cell_measurement_theta_min      2.01
_cell_volume                     4553(2)
_computing_cell_refinement       'SMART SAINT'
_computing_data_collection       SMART
_computing_data_reduction        SAINT
_computing_molecular_graphics    'SHELXP-97 (Sheldrick, 1997)'
_computing_publication_material  'SHELCIF-97 (Sheldrick, 2000)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100(2)
_diffrn_detector_area_resol_mean 0
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker APEXII'
_diffrn_measurement_method       '0.3 wide w/ exposures'
_diffrn_radiation_monochromator  'Quazar optics'
_diffrn_radiation_source         'Imus microdocused'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1178
_diffrn_reflns_av_sigmaI/netI    0.0593
_diffrn_reflns_limit_h_max       19
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            50967
_diffrn_reflns_theta_full        27.53
_diffrn_reflns_theta_max         27.53
_diffrn_reflns_theta_min         2.01
_exptl_absorpt_coefficient_mu    9.436
_exptl_absorpt_correction_T_max  0.790
_exptl_absorpt_correction_T_min  0.642
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   SHELXPREP
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    2.662
_exptl_crystal_density_meas      ?
_exptl_crystal_description       needle-like
_exptl_crystal_F_000             3360
_exptl_crystal_size_max          0.156
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.025
_refine_diff_density_max         1.648
_refine_diff_density_min         -1.407
_refine_diff_density_rms         0.260
_refine_ls_extinction_coef       0.000035(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.007
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     309
_refine_ls_number_reflns         5225
_refine_ls_number_restraints     90
_refine_ls_restrained_S_all      1.000
_refine_ls_R_factor_all          0.0670
_refine_ls_R_factor_gt           0.0377
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0343P)^2^+9.9903P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0713
_refine_ls_wR_factor_ref         0.0809
_reflns_number_gt                3785
_reflns_number_total             5225
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic200006m_si_002_1.cif
_cod_data_source_block           UCePhP2
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'n/a' was changed to '?' - the
value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4325180